Efficiency improvement of silicon solar cells enabled by ZnO nanowhisker array coating
© Yu et al.; licensee Springer. 2012
Received: 6 April 2012
Accepted: 1 June 2012
Published: 15 June 2012
An efficient antireflection coating is critical for the improvement of silicon solar cell performance via increased light coupling. Here, we have grown well-aligned ZnO nanowhisker (NW) arrays on Czochralski silicon solar cells by a seeding-growth two-step process. It is found that the ZnO NWs have a great effect on the macroscopic antireflection effect and, therefore, improves the solar cell performance. The ZnO NW array-coated solar cells display a broadband reflection suppression from 500 to 1,100 nm, and the minimum reflectance smaller than 3% can easily be achieved. By optimizing the time of ZnO NW growth, it has been confirmed that an increase of 3% relatively in the solar cell efficiency can be obtained. These results are quite interesting for the application of ZnO nanostructure in the fabrication of high-efficiency silicon solar cells.
KeywordsSilicon Solar cell Antireflection ZnO nanowhisker Efficiency.
Antireflection (AR) technology plays an important role in the fabrication of high-efficiency solar cells by increasing light coupling into the active region of devices. Generally, a relatively low-light reflectivity can be obtained for crystalline silicon solar cells by combining surface texturization with SixNy-thin-film deposition [1, 2]. However, in order to further reduce the light reflectivity for the improvement of solar cell efficiency, a variety of nanostructures with size comparable to the wavelength of m:most of the utilized solar spectrum have been proposed, such as photonic crystals , porous structures , plasm:monics [5–8], etc. The subwavelength structures can be nanowires , nanocones [10, 11], frustum nanorods , biomimetic nanostructures [13–16], dielectric nanoparticles [17, 18] etc. All these nanostructures should be based on the wide bandgap materials which, themselves, cannot absorb sunlight.
The ZnO material has a wide bandgap, which has been popularly used in the fields of photocatalysis  and optoelectronic nanodevices . For photovoltaic application, the ZnO nanostructures as antireflective layers could be fabricated by various approaches like pulsed laser deposition , chemical vapor deposition , vapor–liquid-solid growth , hydrothermal method , and electrochemical deposition technique . Am:mong them, a seeding and growth two-step process in zinc salt and amide mixed solutions seems quite acceptable for photovoltaics due to its low cost and good potential for scale-up [26, 27]. Experiments have shown that ZnO nanorod arrays can exhibit better antireflective properties than other oxide compounds . A weighted global reflectance of 6.6% has been achieved in the broadband range from 400 to 1,200 nm . However, m:most work on ZnO nanorod arrays as antireflective layers is performed on the naked silicon wafer by now [29, 30]. The application of ZnO nanostructures in the practical silicon solar cells is seldom reported.
In this work, we have grown ZnO nanowhiskers (NWs) with different lengths by the seeding and growth two-step process, and meanwhile have integrated the ZnO NW technique into the fabrication of Czochralski (CZ) silicon solar cells based on the current standard celling technology. The density and the length of ZnO NWs have been optimized for the improvement of solar cell performances by controlling the time of growth. The result shows that the efficiency of CZ silicon solar cell can be improved by a value of 3% relatively using the ZnO NWs as the AR layer in practice.
The starting samples are p-type CZ silicon solar cells fabricated by a standard process including surface texturization, phosphorus diffusion, SixNy film deposition, screen printing, and metallization. The size of solar cells is 4 × 4 cm2. The seed layer of ZnO was first deposited on the front surface of solar cells by a magnetron sputtering system. The deposition temperature is 150°C, and the seed layer thickness is about 10 nm. After protecting the parts without the ZnO seed film with waterproof tapes, the samples were immersed in the solution of zinc nitrate hexahydrate (Zn(NO3)2·6H2O) and (CH2)6 N4 mixture for 30 to 60 min for the growth of ZnO NW. The ZnO NW growth temperature is 90°C.
For characterization, a scanning electron microscope (SEM; Hitachi S-4800, Hitachi, Ltd., Chiyoda, Tokyo, Japan) was used to observe the ZnO NWs on the solar cells. The reflection spectra of the samples were measured by a UV–vis spectrophotometer (Hitachi U-4100) in the wavelength range of 300 to 1,100 nm. The external quantum efficiencies (EQEs) of the final solar cells were obtained from the spectral responses. The current–voltage characteristics of the cells under the dark and illumination circumstances were measured. For illumination, one sun (100 mW/cm2) with AM 1.5 Global spectrum was used.
Results and discussion
Zn2+ is provided by Zn(NO3)2·6H2O through its ionization in the solution. The decomposition of hexamethylenetetramine produces amm:monia that can supply the OH− needed for the ZnO NW formation reaction and acts as a pH buffer to regulate the pH value of the solution . The pH value of the solution should be 6 or 7 for the whole reaction process. During the process, the ZnO nanocrystals existing in the seed layer serve as the nucleation centers where the growth of ZnO NWs takes place. Due to its growth habit, c-axis is the m:most preferred growth orientation , which leads to the formation of ZnO NWs.
Performance parameters of c-Si solar cells with and without ZnO NWs
ZnO growth time (min)
In summary, around 100 to 300 nm ZnO NWs are grown on the surface of Czochralski Si solar cells based on a low cost aqueous solution method. ZnO NWs grown for different times, such as 30, 45, and 60 min, can reduce the reflectivity of the solar cells effectively (R < 3%) in a large spectral region and improve the external quantum efficiency in the corresponding range. Furtherm:more, ZnO NWs with 45-min growth time can improve the efficiency of the solar cells by 3%, corresponding to their increment of short-circuit current density and fill factor. Finally, long-time immersion of solar cells in aqueous solution during the ZnO NW growth process can deteriorate the solar cell performance drastically.
Deren Yang and Xuegong Yu are both professors and doctorate degree holders in the State Key Laboratory of Silicon Materials, Department of Materials Science & Engineering, Zhejiang University. Dong Wang, Dong Lei, and Genhu Li are masters degree holder candidates of the same university.
This work is supported by the National Natural Science Foundation of China (grant nos. 60906002 and 50832006), National Key Technology R&D Program (2011BAE03B13), Key Laboratory of Optoelectronic Materials Chemistry and Physics, CAS (2008DP173016), and Innovation Team Project of Zhejiang Province (2009R50005).
- Green M: Silicon Solar Cells: Advanced Principles and Practice. Bridge, Sydney; 1995.Google Scholar
- Singh P, Kumar R, Lal M, Singh S, Das B: Effectiveness of anisotropic etching of silicon in aqueous alkaline solutions. Sol Energy Mater Sol Cells 2001, 70: 103. 10.1016/S0927-0248(00)00414-1View ArticleGoogle Scholar
- Śmigaj W, Gralak B, Pierre R, Tayeb G: Antireflection gratings for a photonic-crystal flat lens. Opt Lett 2009, 34(22):3532. 10.1364/OL.34.003532View ArticleGoogle Scholar
- Kennedy S, Brett M: Porous broadband antireflection coating by glancing angle deposition. Appl Opt 2003, 42(22):4573. 10.1364/AO.42.004573View ArticleGoogle Scholar
- Ebbesen T, Lezec H, Ghaemi H, Thio T, Wolff P: Extraordinary optical transmission through sub-wavelength hole arrays. Nature 1998, 391: 667. 10.1038/35570View ArticleGoogle Scholar
- Ozbay E: Plasm:monics: merging photonics and electronics at nanoscale dimensions. Science 2006, 311(5758):189. 10.1126/science.1114849View ArticleGoogle Scholar
- Wu J, Mangham Scott C, Reddy VR, Manasreh m:mo, Weaver BD: Surface plasm:mon enhanced intermediate band based quantum dots solar cell. Solar Energy Materials & Solar Cells 2012, 102: 44.View ArticleGoogle Scholar
- Wu J, Makableh YFM, Vasan R, Manasreh m:mo, Liang B, Reyner CJ, Huffaker DL: Strong interband transitions in InAs quantum dots solar cell. Appl Phys Lett 2012, 100: 051907. 10.1063/1.3681360View ArticleGoogle Scholar
- Garnett E, Yang P: Light trapping in silicon nanowire solar cells. Nano Lett 2010, 10: 1082. 10.1021/nl100161zView ArticleGoogle Scholar
- Zhu J, Yu Z, Burkhard GF, Hsu C, Connor S, Xu Y, Wang Q, McGehee M, Fan S, Cui Y: Optical absorption enhancement in am:morphous silicon nanowire and nanocone arrays. Nano Lett 2009, 9(1):279. 10.1021/nl802886yView ArticleGoogle Scholar
- Zhu J, Hsu C, Yu Z, Cui Y: Nanodome solar cells with efficient light management and self-cleaning. Nano Lett 1979, 2010: 10.Google Scholar
- Tsai M, Tseng P, Chen H, Kuo H, Yu P: Enhanced conversion efficiency of a crystalline silicon solar cell with frustum nanorod arrays. Opt Express 2011, 19(S1):A28. 10.1364/OE.19.000A28View ArticleGoogle Scholar
- Linn N, Sun C, Jiang P, Jiang B: Self-assembled biomimetic antireflection coatings. Appl Phys Lett 2007, 91: 101108. 10.1063/1.2783475View ArticleGoogle Scholar
- Min W, Jiang B, Jiang P: Bioinspired self‒cleaning antireflection coatings. Adv Mater 2008, 20(20):3914. 10.1002/adma.200800791View ArticleGoogle Scholar
- Song Y, Jang S, Yu J, Lee Y: Bioinspired parabola subwavelength structures for improved broadband antireflection. Small 2010, 6(9):984. 10.1002/smll.201000079View ArticleGoogle Scholar
- Sun C, Jiang P, Jiang B: Broadband m:moth-eye antireflection coatings on silicon. Appl Phys Lett 2008, 92: 061112. 10.1063/1.2870080View ArticleGoogle Scholar
- Akim:mov Y, Koh W, Sian S, Ren S: Nanoparticle-enhanced thin film solar cells: metallic or dielectric nanoparticles. Appl Phys Lett 2010, 96: 073111. 10.1063/1.3315942View ArticleGoogle Scholar
- Huang C, Lin H, Chen J, Sun K, Chang W: Efficiency enhancement of the poly-silicon solar cell using self-assembled dielectric nanoparticles. Sol Energy Mater Sol Cells 2011, 95(8):2540. 10.1016/j.solmat.2011.03.006View ArticleGoogle Scholar
- Ma C, Zhou Z, Wei H, Yang Z, Wang Z, Zhang Y: Rapid large-scale preparation of ZnO nanowires for photocatalytic application. Nano Res Lett 2011, 6: 536. 10.1186/1556-276X-6-536View ArticleGoogle Scholar
- Zhou Z, Zhan C, Wang Y, Su Y, Yang Z, Zhang Y: Rapid mass production of ZnO nanowires by a m:modified carbothermal reduction method. Mater Lett 2011, 65: 832. 10.1016/j.matlet.2010.12.032View ArticleGoogle Scholar
- Kawakami M, Hartanto A, Nakata Y, Okada T: Synthesis of ZnO nanorods by nanoparticle assisted pulsed-laser deposition. Jpn J Appl Phys 2003, 42: L33. 10.1143/JJAP.42.L33View ArticleGoogle Scholar
- Wu J, Liu S: Low-temperature growth of well-aligned ZnO nanorods by chemical vapor deposition. Adv Mater 2002, 14: 215. 10.1002/1521-4095(20020205)14:3<215::AID-ADMA215>3.0.CO;2-JView ArticleGoogle Scholar
- Huang M, Mao S, Feick H, Yan H, Wu Y, Kind H, Weber E, Russo R, Yang P: Room-temperature ultraviolet nanowire nanolasers. Science 1897, 2001: 292.Google Scholar
- Yamabi S, Imai H: Growth conditions for wurtzite zinc oxide films in aqueous solutions. J Mater Chem 2002, 12: 3773. 10.1039/b205384eView ArticleGoogle Scholar
- Liu R, Vertegel A, Bohannan E, Sorenson T, Switzer J: Epitaxial electrodeposition of zinc oxide nanopillars on single-crystal gold. Chem Mater 2001, 13: 508. 10.1021/cm000763lView ArticleGoogle Scholar
- Greene L, Law M, Goldberger J, Kim F, Johnson J, Zhang Y, Saykally R, Yang P: Low‒temperature wafer‒scale production of ZnO nanowire arrays. Angew Chem Int Edn 2003, 42: 3031. 10.1002/anie.200351461View ArticleGoogle Scholar
- Vayssieres L, Keis K, Hagfeldt A, Lindquist S: Three-dimensional array of highly oriented crystalline ZnO microtubes. Chem Mater 2001, 13: 4395. 10.1021/cm011160sView ArticleGoogle Scholar
- Takato H, Yamanaka M, Hayashi Y, Shim:mokawa R, Hide I, Gohda S, Nagamine F, Tsuboi H: Effects of optical confinement in textured antireflection coating using ZnO films for solar cells. Jpn J Appl Phys 1992, 31: L1665. 10.1143/JJAP.31.L1665View ArticleGoogle Scholar
- Lee Y, Ruby D, Peters D, McKenzie B, Hsu J: ZnO nanostructures as efficient antireflection layers in solar cells. Nano Lett 2008, 8: 1501. 10.1021/nl080659jView ArticleGoogle Scholar
- Ghong T, Kim Y, Ahn E, Yoon E, An S, Yi G: Application of spectral reflectance to the m:monitoring of ZnO nanorod growth. Appl Surf Sci 2008, 255: 746. 10.1016/j.apsusc.2008.07.048View ArticleGoogle Scholar
- Vayssieres L, Keis K, Lindquist S, Hagfeldt A: Purpose-built anisotropic metal oxide material: 3D highly oriented microrod array of ZnO. J Phys Chem B 2001, 105: 3350. 10.1021/jp010026sView ArticleGoogle Scholar
- Govender K, Boyle D, Kenway P, Brien P: Understanding the factors that govern the deposition and m:morphology of thin films of ZnO from aqueous solution. J Mater Chem 2004, 14: 2575. 10.1039/b404784bView ArticleGoogle Scholar
- Wang ZL: Nanostructures of zinc oxide. Mater Today 2004, 7: 26.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Comm:mons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.